Temperature-Sensitive Poly(vinyl alcohol)/Poly(methacrylate-co-N-isopropyl acrylamide) Microgels for
Shivkumar V. Ghugare, Pamela Mozetic, and Gaio Paradossi*
Dipartimento di Scienze e Tecnologie Chimiche, and CRS SOFT CNR-INFM, Universita di Roma TorVergata, 000133 Roma, Italy
Received February 11, 2009; Revised Manuscript Received April 8, 2009
Microgels based on poly(vinyl alcohol), PVA, grafted with methacrylate side chains, MA, incorporatingN-isopropylacrylamide, NiPAAm, monomer, were prepared by water-in-water emulsion polymerization method.These systems exhibit a spherical shape and a volume-phase transition, that is, shrinking, below physiologicaltemperature. The behavior of these microgels were studied with respect to their average size and size distribution,swelling, and release properties. It was observed that the stirring speed is a key parameter for controlling theamount of incorporated NiPAAm, the particle size and the sharpness of the volume-phase transition. The volume-phase transition temperature, VPPT, of the microgels was evaluated around 38 and 34 C for microgels with aNiPAAm/methacrylate molar ratio of 0.8 and 2.4, respectively. Water uptake increased with the amount of NiPAAmmonomer present in the polymer network. In vitro biocompatibility of microgels was assessed with respect toNIH3T3 mouse fibroblasts. O-Succinoylated microgels were loaded with doxorubicin by exploiting the favorableelectrostatic interaction between negatively charged microgel surface and positively charged doxorubicin. Thedrug release was influenced by the microgels surface/volume ratio. At physiological temperatures, above theVPTT exhibited by these systems, the release was enhanced by the specific area increase. This study providesthe background for the design of an injectable device suitable for the controlled delivery of doxorubicin based onthe volume-phase transition of microgels.
Fast response to external parameters is what makes a systemintelligent.1,2 Design of the properties and functions of devicessensible to external gradients involves a number of differentstructural and dynamic parameters.3 In the case of polymerhydrogels, the main contribution to the response is a volumetransition that can be triggered by pH, ionic strength, andtemperature.47 Responsivity to these stimuli are largely ampli-fied by the connectivity characterizing a chemically cross-linkedhydrogel. The presence of fixed and ionizable charges in thepolymer network makes possible the triggering by pH and ionicstrength, whereas the temperature transition is caused by thepresence of residues displaying a thermally sensible behaviorin the polymer network due to the interpolymer chain associationthrough hydrophobic interaction. Focusing on networks featuringthis latter effect, the choice of possible monomers to use asbuilding blocks of the responsive polymer network is greatlylimited by environment and temperature conditions in whichthe device is designed to function. When responsivity iscombined with a high value of specific surface, exchangeprocesses will be largely enhanced.4,811 This can be achievedby colloidal microdevices such as microgels, where a favorablelarge surface/volume ratio can enhance the bioavailability ofthe drug playload.12
The microgel particles are designed as injectable drugdeliverable systems for parenteral administration. For this kindof application, requirements are the nano/micro overall size anda large water volume fraction to preserve the conformationalstate of the drug payload.811,13
The interaction with cells is one of the processes occurringas soon as the microgels are injected in the bloodstream.14
Devices based on soft matter are attractive because of theirunique chemical and physical versatility for conjugating mol-ecules able to promote adhesion to targeted cells and to allowlocal drug delivery. However, this suitability is counterbalancedby the general requirements involving biocompatibility of thematerial used for designing the sphere microgels.
The use of NiPAAm as a key monomer for assigning thermalresponsivity to the network has been often made. The lowercritical solution temperature, LCST, occurring in poly(NiPAAm)aqueous solution around 32 C,15 is at the base of a volume-phase transition displayed in hydrogels containing cross-linkedpoly(NiPAAm) and has been used to design the organiccomponent in hybrid devices incorporating quantum dots.16
Recently, the structure of poly(NiPAAm) microgels in aqueoussuspensions has been determined.17,18 The dynamics of thepolymer chains around the transition temperature19 and of thesolvent confined in the network20 have been investigated byincoherent quasi elastic neutron scattering and by NMR 1Hspin-spin relaxation time measurements, respectively.
The temperature transition is influenced by factors as pH,ionic strength, and presence of comonomers. However, in manycases, VPTT is close or coincident with physiological temper-ature conditions.21 This background suggests that loaded nano/micro systems could undergo significant size changes with anefficient release of the drug payload making microgels attractivefor the design of injectable devices with tailored features.
Our previous experience in fabrication of microgels22 withgood colloidal stability based on a methacryloyl-derivatizedpoly(vinyl alcohol) network23 by water-in-water microemulsionsprovided the background for incorporating NiPAAm in the
* To whom correspondence should be addressed. E-mail: firstname.lastname@example.org.
Biomacromolecules 2009, 10, 15891596 1589
10.1021/bm900185u CCC: $40.75 2009 American Chemical SocietyPublished on Web 05/08/2009
network to obtain thermal responsivity to the resulting microgels.It should be stressed that this water-in-water microemulsionpolymerization has the remarkable advantage to use nontoxicchemicals throughout the synthesis. This assures that theresulting microgels will not release harmful molecules duringtheir functioning. Moreover, the use of a poly(vinyl alcohol),PVA, based drug delivery microgels should allow for a low, ifany, cytotoxic impact on cells.
We addressed this work to the design of smart, that is, stimuli-responsive, drug delivery microgels, testing their biocompat-ibility and ability to control the drug release with an anticancercase molecule as doxorubicin.
Thermal response of the microgels can also be consideredfor the design of nano/micro temperature sensors as it will beillustrated in a next paper. Here we focus on the structural andthermal features of PVA/Poly(MAmNiPAAmn) microgels.
Materials. N-Isopropyl acrylamide (NiPAAm), purchased fromAldrich chemicals, was recrystallized in n-hexane prior to use. All otherchemicals were used as received. Poly(vinyl alcohol) with number andweight average molecular weights of 30000 ( 5000 and 70000 ( 10000g/mol, respectively, dextranT40 and blue dextran, with a numberaverage molecular weight of 35000-40000 and 2000000 g/molrespectively, succinic anhydride and phosphate-buffered saline (PBS)were purchased from Sigma.
4-(N,N-Dimethylamino) pyridine (DMAP), glycidylmethacrylate(GMA), and fluorescein isothiocynate isomer 1 (FITC) were Flukaproducts. Photoinitiator 2-hydroxy-1-[4-(hydroxyethoxy)phenol]-2-methyl 1-propanone (Irgacure 2959) was purchased from Ciba.
Dimethyl sulfoxide (DMSO), inorganic acids, and bases were RPEgrade products supplied by Carlo Erba.
Dulbeccos modified Eagles medium (DMEM), L-glutamine 200mM, and penicillin/streptomycin solution, at a concentration of 10000U/mL and 10 mg/mL, respectively, were purchased from HyClone.Fetal bovine serum and MTT (3-(4,5-dimethylthyazol-2-yl)-2,5-diphe-nyltetrazolium bromide) were Sigma products.
Water was Milli-Q purity grade (18.2 M cm) produced with adeionization apparatus (PureLab) from USF, Elga. Dialysis membranes(cut off 12000 g/mol) were purchased from Medicell International Ltd.and prepared according to standard procedure.
Methods. Synthesis of Poly(Vinyl alcohol)-methacrylate (PVA-MA).PVA was grafted with glycidylmethacrylate according to the proceduredescribed elsewhere.2426 Briefly, 10 g of PVA was dissolved in 250mL of DMSO at 70 C. After complete dissolution of PVA, the flaskwas cooled to room temperature, and then 5 g DMAP was added underN2 flux. After 1 h, a known amount of GMA was added in the propermolar ratio with respect to polymer repeating unit. The reaction wascarried out at room temperature in darkness with stirring and stoppedafter 48 h by neutralizing the solution with an equal molar amount ofHCl with respect to DMAP. DMSO was replaced with water byexhaustive dialysis. The sample was stored as a freeze-dried powder.After methacryloyl grafting, the degree of substitution (DS) wasdetermined by 1H NMR analysis.24 For microgel preparation, a samplewith DS 4.7%, hereafter labeled PM5, was used throughout this study.
Preparation of Microgels. Microgels based on PM5 were prepared,adapting a procedure originally introduced by Franssen and Hennink,22,27
which employs a water-in-water emulsion technique based onpolymer-polymer immiscibility in aqueous solutions. In a typicalexperiment, an aqueous dispersion containing dextran T40 at aconcentration of 16% (w/v), PM5 at 2% (w/v), and the UV photoini-tiator Irgacure 2959 at 0.3% (w/v) was vigorously